• FIRE RESISTANCE OF HSC
• EFFECT OF FIRE ON NSC
• FACRORS GOVERNING THE FIRE PERFORMANCE OF HSC
• EXPERIMENTAL STUDIES
• PARAMETERS AFFECTED BY FIRE
WHAT IS HSC?
• It is a type of high performance concrete generally with a
specified compressive strength of 40 Mpa or greater.
• The compressive strength is measured at 56 days or 90 days
or some other specified age depending upon the application.
• To put the concrete at service at much earlier age.
• To build high rise buildings by reducing column sizes and
increasing available space.
• To build the superstructure of long-span bridges and to
enhance the durability of bridge decks.
WHY DO WE NEED HSC?
• In recent years, the construction industry has shown more interest
in the use of high strength concrete (HSC).
• This is due to the improvements in structural performance, such as
high strength and durability, that it can provide compared to normal
strength concrete (NSC).
• Recently, the use of high strength concrete, which was previously in
applications such as bridges, off-shore structures and infrastructure
projects, has been extended to high rise buildings.
• One of the major uses of HSC in buildings is for columns.
•The dimensions of the column cross section and
other specifics of the columns are given in Table 1.
• Columns HSC1 and HSC2 had eight, 20 mm, longitudinal bars,
while Column NSC1 had four, 20 mm, longitudinal bars.
• In the HSC columns, the bars were tied with 10 mm ties at a
spacing of 225 mm; while in the NSC columns, the bars were
tied with 8 mm ties at a spacing of 305 mm.
• The main reinforcing bars and ties had a specified yield
strength of 400 MPa.
• Three batches of concrete were used in fabricating the
• The mix for Batch 1 and Batch 2 used HSC, while the mix for
Batch 3 used NSC.
• The coarse aggregate in Batches 1 and 3 was carbonate while
in Batch 2 it was siliceous aggregate.
• Columns HSC1, HSC2 and NSC1 were fabricated from Batch 1,
Batch 2 and Batch 3, respectively.
• The moisture condition at the centre of the column was also
measured on the day of the test.
• The moisture conditions of Columns HSC1, HSC2 and NSC1 are
approximately equivalent to those in equilibrium with air of
69% relative humidity (RH), 63% RH and 75% RH, respectively,
at room temperature.
• The tests were carried out by exposing the columns to heat in
a furnace specially built for testing loaded columns.
• The furnace consists of a steel framework supported by four
steel columns, with the furnace chamber inside the
• The test furnace was designed to produce conditions, such as
temperature, structural loads and heat transfer, to which a
member might be exposed during a fire.
• The furnace has a loading capacity of 1,000 t.
TEST CONDITION AND PROCEDURE
• The columns were installed in the furnace by bolting the
endplates to a loading head at the top and to a hydraulic jack
at the bottom.
• The conditions of the columns were fixed-fixed for all tests.
• For each column, the length exposed to fire was
approximately 3000 mm.
• For columns tested fixed at the ends, an effective length of
2000 mm represents experimental behaviour.
• Column HSC1 was subjected to a load of 2000 KN.
• Column HSC2 was subjected a load of 1700 KN.
• Column NSC1 to a load of 1067 KN.
• The load was applied approximately 45 min before the start of
the fire test and was maintained until a condition was reached
at which no further increase of the axial deformation could be
• The load was maintained constant throughout the test.
RESULTS AND DISCUSSION
• The temperature-time curves for the external surface and for
various depths in concrete are plotted.
• For all three columns, the temperatures inside the column
rose rapidly to about 100°C and then the rate of increase of
• Both the NSC and HSC columns expanded until the
reinforcement yielded and then contracted leading to failure.
• It can be seen that deformation in the HSC columns was
slightly less than that for the NSC column.
• The deformation in the columns resulted from several factors,
such as load, thermal expansion and creep.
• Initial deformation of the column was mainly due to the
thermal expansion of concrete and steel.
• While the effect of load and thermal expansion is significant in
the intermediate stages, the effect of creep becomes
pronounced in the later stages due to the high fire
• This is one of the main reasons that the deformations are
quite large before the failure of the columns.
• All three columns failed in compression mode.
• In the NSC column, no significant spalling occurred until the
failure of the column.
• In the case of HSC columns, there was noticeable spalling at
the end of the test.
• The cracks in these HSC columns progressed at the corners of
the cross section, with the increase in time, and led to spalling
of chunks of concrete.
• This spalling was significant at about mid-height.
• While minute cracks could be noticed in about 20 to 30 min,
the widening of these cracks occurred after about 60 min or
• In the case of Column HSC1 (carbonate aggregate concrete),
the spalling was less compared to Column HSC2 (siliceous
• This could be attributed to the effect of aggregate used in the
concrete mix and also to the intensity of load.
• For the NSC column, the fire resistance was approximately
• For Columns HSC1 and HSC2, it was 225 and 189 min,
• High-strength concrete is a high-performing material that
offers a number of advantages. Engineers can enhance its fire
performance by adopting the following guidelines:
– Use normal-weight aggregate (instead of lightweight
aggregate) to minimize spalling.
– Add polypropylene fibres to the mix to reduce spalling.
– Add steel fibres to enhance tensile strength and reduce
– Use carbonate aggregate (instead of siliceous aggregate) to
– Employ both closer tie spacing and cross ties to improve
– Install bent ties (at 135° back into the concrete core)
instead of straight ties.
– Take appropriate precautions to prevent spalling when
concrete strength exceeds 55 MPa.